Full Terms & Conditions of access and use can be found at
ISSN: (Print) (Online) Journal homepage: https://www.tandfonline.com/loi/kbie20
Removal of hydrogen sulfide from biogas using
activated carbon synthesized from different locally
available biomass wastes - a case study from
Hassan Sawalha , Maher Maghalseh , Janna Qutaina , Kholoud Junaidi & Eldon R. Rene
To cite this article: Hassan Sawalha , Maher Maghalseh , Janna Qutaina , Kholoud Junaidi & Eldon R. Rene (2020) Removal of hydrogen sulfide from biogas using activated carbon synthesized from different locally available biomass wastes - a case study from Palestine, Bioengineered, 11:1, 607-618, DOI: 10.1080/21655979.2020.1768736
To link to this article: https://doi.org/10.1080/21655979.2020.1768736
© 2020 The Author(s). Published by Informa UK Limited, trading as Taylor & Francis Group.
Published online: 28 May 2020.
Submit your article to this journal
Article views: 1501
View related articles
Removal of hydrogen sulfide from biogas using activated carbon synthesized
from different locally available biomass wastes - a case study from Palestine
Hassan Sawalha a, Maher Maghalsehb, Janna Qutainaa, Kholoud Junaidia, and Eldon R. Renec
aRenewable Energy and Environment Research Unit, Mechanical Engineering Department, Palestine Polytechnic University, Hebron, Palestine; bRenewable Energy and Environment Research Unit, Electrical Engineering Department, Palestine Polytechnic University, Hebron, Palestine; cDepartment of Environmental Engineering and Water Technology, IHE Delft Institute for Water Education, Delft, The Netherlands
The main aim of this study was to remove hydrogen sulfide (H2S) from biogas by adsorption using synthesized activated carbon prepared using locally available biomass. The effect of the type of precursors, impregnation reagent and bed height was studied in continuous reactors. Three types of biomass wastes (almond shells, eucalyptus and coffee grains) were collected, grinded, sieved, pyrolyzed at 500°C and impregnated with chemical reagents such as potassium hydroxide or zinc chloride. Adsorption tests were performed using a fixed bed filter filled with the produced activated carbon. The highest biochar yield of 36% was obtained eucalyptus followed by almond shells (28.5%) and coffee grains (24%), respectively. The highest adsorption capacity and removal efficiency were obtained with eucalyptus followed by almond shells and coffee grains, respec-tively. For instance, eucalyptus showed an adsorption capacity of ~690 (mg hydrogen sulfide/g adsorbent) followed by almond (230 mg hydrogen sulfide/g adsorbent) and coffee grains (22 mg hydrogen sulfide/g adsorbent). As an impregnation reagent, potassium hydroxide gave the high-est adsorption efficiency and capacity than zinc chloride. Furthermore, the breakthrough time with KOH (180 min) was higher than ZnCl2(70 min). Increasing the bed height during continuous breakthrough tests increased the adsorption capacity and hydrogen sulfide removal efficiency. The results of this study showed that the adsorption efficiency of the synthesized activated carbon and consequently the hydrogen sulfide removal efficiency could be fine-tuned by selecting an appropriate biomass precursor and proper impregnation reagent.
ARTICLE HISTORY Received 26 February 2020 Revised 27 April 2020 Accepted 27 April 2020 KEYWORDS Hydrogen sulfide; packed-bed; adsorption; activated carbon; removal efficiency
Biogas is a promising renewable energy source that can replace the conventionally used nonrenewable fossil fuels in most of the developing countries (e.g. Palestine and India). Conventionally, biogas is com-monly produced through the anaerobic digestion of
different biomass feedstocks including animal, agri-cultural and organic food waste resides [1–5]. The produced biogas is mainly composed of methane, carbon dioxide and fractions of water vapor and hydrogen sulfide (H2S), i.e. H2S is an impurity of biogas . The presence of H2S adversely affects the
CONTACTHassan Sawalha firstname.lastname@example.org Renewable Energy and Environment Research Unit, Mechanical Engineering Department, Palestine Polytechnic University, P.O. Box: 198, Wadi Al-Haria, Hebron, Palestine
2020, VOL. 11, NO. 1, 607–618
© 2020 The Author(s). Published by Informa UK Limited, trading as Taylor & Francis Group.
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
quality of the biogas and it has major environmental and technical drawbacks. For instance, at concentra-tions of 1000 to 2000 ppm, H2S can cause a collapse, coma and death from respiratory failure within a few seconds after one or two inhalations . At concen-trations of 100 to 200 ppm, H2S may cause a blurred vision and death following exposure for 1–8 h . Moreover, dissolved H2S with concentration up to 50 ppm causes fermentation inhibition since it is toxic to the bacteria in the slurry of bioreactors . Technically, H2S is corrosive and can significantly damage the metallic parts of the biogas facilities and electrical generator . Furthermore, the electrical generation efficiency dramatically decreases when the H2S concentration in the biogas is very high. From an environmental perspective, the combustion of H2S during electrical generation forms sulfur dioxide (SO2), leading to the formation of a highly corrosive gas and it contributes as a major source of acid rains . Therefore, the removal of H2S form the biogas is of high technical, environmental and health importance.
In the literatures, various biological, chemical and physical techniques have been successfully applied for the purification of biogas from H2S such as biological desulfurization, chemical absorption, water scrubbing, membranes and adsorption [8– 14]. Adsorption is one of the most effective technol-ogies applied in removing H2S from biogas streams. The high H2S removal efficiency achieved by adsorp-tion makes it superior over other purificaadsorp-tion tech-niques. Besides, it is a rather inexpensive technique with wide range of choices of low-cost adsorbents.
During the adsorption process, the biogas is contacted with an adsorbent in which the H2S is collected on the surface and interior microstruc-ture of the adsorbent. Several types of adsorbents have been proposed in the literature, including metal oxides, silica gel, zeolites, synthetic resins, and activated carbon [8,15–21]. Activated carbon has been widely used for the treatment of waste-water and waste gases. The high porosity and surface area of activated carbon provide a high capacity for the separation of pollutants from the liquids and gases present in the polluted envir-onment. The activated carbon is commonly pro-duced through the pyrolysis and impregnation of various biomass feedstock . During pyrolysis, the biomass is thermally decomposed in the
absence of oxygen at a controlled temperature to produce biochar . The biochar, also called
‘charcoal’ in the literature, is the solid product from pyrolysis, or it is the carbonaceous residue after all the volatile matter leaves the biomass as gases and tar. The pyrolysis process is usually followed by an impregnation step. There are three types of activation: physical, chemical and physico-chemical activation .
Chemical impregnation is largely implemented in practice due to the lower impregnation temperatures and shorter treatment time compared to other impregnation methods; besides, it offers a larger sur-face area, microporosity and yield of the obtained activated carbon (AC) . In chemical impregna-tion, the carbonized char material is impregnated with an oxidizing agent for dehydration by mixing or kneading with a concentrated solution of acid or base. The impregnation procedure increases the por-osity and surface area and widens the existing micro-pores and mesomicro-pores of the char matrix . The internal surface area of the AC can reach values up to 500 to 1500 m2/g . The common chemical reagents applied at the industrial scale for the impregnation of biochar include ZnCl2, H3PO4, NaOH, KOH, and K2CO3[24,27].
It is worth mentioning that the properties of the produced AC strongly depend on the type of pre-cursor biomass and the operating conditions during pyrolysis (Ahmad et al., 2019). The lignin and cel-lulose content of the plant texture greatly affects the microstructure of the produced AC. Previous stu-dies have shown that, the higher the lignin content in the biomass, the higher the biochar yield and micropores surface area . In addition, the oper-ating conditions, including temperature and pyro-lysis residence time, play an important role in the yield and quality of the biochar produced. Generally, when conducting the pyrolysis at low temperatures (~500oC), high residence time is favorable for producing high-quality biochar . Most of the previous adsorption studies in the lit-erature have mainly focused on wastewater treat-ment; however, biogas purification using biochar adsorbents was lightly investigated.
Concerning the novelty of this work, in Palestine, the biogas production is quite limited, with only one full scale industrial-scale biogas plant that is in operation. In this plant, cow
manure is being used as a feedstock to the biodi-gester. The generated biogas is purified from H2 S using an expensive commercial AC filter. This study responds to a real need of the biogas indus-try in the counindus-try to provide a relatively cheap biogas purification technology that can also be applied in other developing countries in Asia, Africa and South America. Thus, it is hypothesized that the expensive AC can be replaced with differ-ent low-cost and effective ACs that can be pro-duced from widely available biomass wastes such as spent coffee grains, eucalyptus barks and almond shells. The objective of the present study was to prepare low-cost biochar adsorbents from locally available biomass wastes for application in the purification of biogas from H2S using packed-bed adsorption system. The effect of the type of precursor biomass waste, impregnation agent and the packed-bed characteristics on the H2S removal efficiency was tested in this study.
2. Experimental: materials and methods
2.1. Biomass precursors and biogas composition
Coffee grains (COF) waste was collected from a local home kitchen (Hebron, Palestine). Eucalyptus barks (EUC) and almond shells (ALM) were collected from a local home garden (Hebron, Palestine). Concerning impregnation agents, potassium hydroxide (KOH) and zinc chloride (ZnCl2) (90%, Albemarle, Louisiana, Florida, USA) were used in this study. Biogas was obtained from the Jebrini biogas facility, Al-Dhaheria, Hebron, Palestine. The composition of the biogas stream was as follows: 67.30% CH4, 31.90% CO2, 0.20% O2, 0.07% H2S, 0.53% other minor gases. The biodigester was fed with biomass waste obtained from Al-Jebrini cow farm Al-Dhaheria, Hebron. It con-sists of 20 ton/day of solid cow manure and 60 ton/day of liquid manure mixture (i.e. the solid cow manure mixed with wastewater from the milking station).
2.2. Pretreatment and pyrolysis of biomass wastes
The collected biomass wastes were washed with tap water to remove the impurities and dried in an oven (Daihan LabTech Co., Ltd., South Korea), at 105°C for 24 h. The samples were, then, smashed
and sieved for 15 min using an auto sieve analysis shaker (Matest, Italy) with meshes # (10, 18, 40, 60 and 140). Particles retained on mesh #140 were used for subsequent analysis. The collected particles were filled in a tightly closed porcelain crucible, in order to isolate the oxygen and water vapor, and pyrolyzed at 500°C for 1 h inside a muffle furnace (labTech International Ltd. East Sussex, UK). The yield of the pyrolyzed materials was defined as the ratio of the weight of the produced biochar to the original biomass weight. Most of the samples were tested in triplicate for yield measurements and the average values are presented in this study with their standard deviation values (i.e. the SD, ± values).
For the impregnation of the samples, distilled water was added to the pyrolyzed biomass at a ratio of 10:1 (v/w) (Vwater:wbiomass) and the impregnation reagent was then gradually added into the mixture, at a ratio of 1:4 (wtreagent: wt biomass). The mixture was carefully stirred at 300 rpm and heated to a temperature of 80°C using a hotplate magnetic stirrer (labTech International Ltd. East Sussex, UK) until most of the liquid was evaporated. The sam-ples were then dried in an oven, at 105°C for 24 h.
2.4. Adsorption studies in a packed-bed reactor and flow characteristics studies
Adsorption experiments were performed using a packed-bed plastic filter with an internal diameter of 1 cm and a height of 12 cm (Figure 1). Two thin layers of a porous cloth were placed at the inlet and outlet of the filter in order to hold the AC particles. The bed was firstly run empty (without AC) in order to test the effect of the bed material and closing the cloth on the H2S adsorption behavior. The AC par-ticles were then packed inside the bed at different heights of 2, 4, 6 and 8 cm, respectively. The biogas stream with an average H2S concentration of 970 ppm entered from the top of the filter bed and it was passed through the AC particles before leaving from the bottom of the packed bed reactor. The inlet and outlet concentrations of H2S were recorded dur-ing different time intervals. The removal efficiency of H2S was studied in terms of time course profiles, i.e. by sampling both the inlet and the outlet H2
S concentrations. Thus, the breakthrough curves of the H2S adsorption inside the packed-bed were established by plotting the ratio of the outlet con-centration to the initial concon-centration ratio (c/co) as a function of the operational time.
The biogas flow rate was measured using the water displacement method  and was kept constant at approximately 1.5–1.7 L/min. The flow through the bed was characterized by estimating the Reynold’s number of the flow, as given in Equation (1) . The bed characteristics and operating conditions are listed inTables 1and2, respectively.
Rep ¼ ρU D 1ε
ð Þμ (1)
whereρis the gas density (Kg/m3),Uis the super-ficial fluid velocity through the bed (m/s),Dis the bed diameter (m),μ is the fluid dynamic viscosity (pa.s), andєis the void fraction of the bed (dimen-sionless). The values of ε were determined using Equation (2):
whereVVis the void volume, which was measured using the fluid saturation method , and VT is total volume of the packed-bed.
The pressure drop for the flow through the bed was calculated using the Carman–Kozeny equation , as follows: Δp H ¼180 μU x2 1ε ð Þ2 ε3 þ1:75 ρU 2 x ð1εÞ ε3 (3)
whereΔpis the pressure drop (pa),His the height of the bed (m), andx is the particle diameter (m).
2.5. Adsorption capacity
The total amount of H2S adsorbed onto the AC particles was determined by applying mass balance principles on the packed-bed, as shown in Figure 2. The general mass balance equation given in Equation (4) was applied.
Total H2 Saccumulation
i:e:total amount of adsorbed H2S
Rate of accumulation Rð Þ
¼ ðcoQÞ ðcQÞ (5)
Figure 1.Experimental setup used for H2S adsorption test
(1,3–inlet and outlet connections, 2–packed bed).
Table 1.The packed bed, biogas characteristics, and operating conditions.
Variable Symbol Value Unit
Density (biogas) ρ 1.17 kg/m3
Dynamic viscosity (biogas) µ 1.26 × 10–5 Pa.s
Flow rate Q 1.5 L/min
Particles average diameter x 177 × 10–6 m
Bed cross-sectional area A 7.85 × 10–5 m2
Superficial velocity U 0.318 m/s
Table 2.Void fraction and pressure drop for the adsorption bed packed with various types of biochar.
Biochar є Rep ΔP/H (kpa/m) ΔP (kpa)
EUC 0.7 984.28 7.01 0.14
ALM 0.63 798.07 14.23 0.28
where co is the inlet concentration of H2S (g/L), cis the outlet concentration of H2S (g/L) and Qis the flow rate (m3/min).
ð1 0 Rdt¼ ð1 0 ð coQcQÞdt (6) ð1 0 Rdt¼Qco ð1 0 ðcoc co Þ dt (7) Total accumulation ¼ ð0 1ð1 c coÞ dt (8)
wheret is the adsorption time (min). The integral
coÞdt in Equation (8) can be obtained from the shaded area of the breakthrough curve as shown in Figure 3.
The adsorption capacity of AC can be obtained from Equation (9) as follows:
whereqis the adsorption capacity of AC (mg H2S/g AC), mH2S is the total amount of H2S (mg) accu-mulated as given in Equation (8) and mAC is the mass of AC (g) filled in the adsorption bed.
3. Results and discussion
3.1. Biochar yield
The yield of the produced biochar from the pyr-olysis process was determined for the three types of biomass waste and the results are shown in Table 3. The highest yield of 36% w/w was obtained with EUC followed by ALM (28.5%) and COF (24%), respectively. The difference in the yield of the biochar might be ascribed to the difference in the lignin and cellulose content; the higher the lignin content, the higher the yield . Therefore, the EUC showed the highest yield due
Figure 2.Activated carbon-based packed bed (CandQare the H2S concentration and flow rate, respectively).
Figure 3.Breakthrough curve achieved after H2S adsorption.
Table 3.The yield, H2S adsorption capacity, and cellulose and
lignin contents of various biochar types.
Biomass Yield (%) Adsorption capacity (mg H2S/g AC) Lignin content (%w/w) Cellulose content (%w/w) Reference EUC 36 (±3.13) 490 26–33 55–68  ALM 28.5 (±0.71) 230 24.8 58  COF 23.87 (±1.96) 22 23.9 51 
to the fact that its lignin content is the highest among others (Table 3) [7,32,33].
3.2. Effect of biomass precursor type on the adsorption characteristics
The effect of the type of biomass waste on the adsorption of H2S was investigated. Figure 4 shows the breakthrough curves of H2S adsorption with an empty bed and when the bed was packed with 2 cm of EUC, ALM and COF biochar acti-vated with KOH, respectively. As seen from the results, when the bed was empty, the breakthrough curve was very steep and the outlet concentration rapidly increased to reach its inlet concentration within about 45 s; indicating that the amount H2 S adsorbed onto the cloth and bed material is almost negligible. On the other hand, when the bed was charged with the AC material, the break-through time dramatically increased compared with those observed when the bed was empty and was highly dependent on the type of biomass precursor material used. At the beginning of the adsorption process, the outlet H2S concentration dramatically dropped to less than 10 ppm for the three samples; indicating high adsorption (H2 S removal) efficiencies. However, with operational time, the outlet H2S concentration increased at different rates depending on the AC sample tested in this study. For instance, with COF, the break-through curve was steeper than EUC and ALM. The outlet concentration remained around zero
(i.e. 100% removal efficiency) for about 3 min and the H2S outlet concentration rapidly increased to reach its inlet concentration after only 10 min. The ALM performed better than the COF; as the outlet concentration remained around zero for about 7 min; thereafter, it gradually increased to reach to its inlet concentration after 130 min (Figure 4).
The highest removal efficiency was observed with EUC as the outlet concentration remained almost zero, with a removal efficiency of about 100% for 45 min. However, after that, it slowly increased to reach its initial value after 180 min. The adsorption capacity of the AC to the H2S, as defined in Equation (9), was calculated for the three types of biomass precursors as shown in Table 3. As seen from the results, the high adsorption capacity observed in this study indicated better adsorption performance. The EUC showed the highest adsorp-tion capacity of about 690 (mg H2S/g AC) followed by ALM and COF, respectively. The difference in the adsorption efficiencies and capacities of H2 S with respect to the type of AC might be explained as follows: The porosity and microstructure of AC are usually strongly affected by the original plant texture, i.e. its lignin and cellulose contents. The lignin content is responsible for the formation of macropores of AC, whereas the cellulose content is mainly responsible for micropores formation . The porosity of the AC obtained from COF (both types micro- and macro-porous) is, therefore, expected to be lower than EUC and ALM, due to
0 0.2 0.4 0.6 0.8 1 0 40 80 120 160 200 c/c o of H 2 S Time (min) Alm Euc Cof empty filter
Figure 4.Breakthrough curves of H2S adsorption in packed bed of EUC, ALM, COF activated with KOH and empty filter. The
experiments were performed at ambient air temperature, gas flow rate (1.5 L/min), bed height (2 cm) and H2S inlet concentration
the fact that it has a lower content of cellulose and lignin than EUC and ALM, respectively. This explains the lower adsorption capacity of the COF compared with the other ACs tested in this study. On the other hand, the EUC has the highest cellu-lose and lignin contents (Table 3) and thereby, one would assume its porosity to be the highest among others, which consequently, rendered the highest adsorption efficiency and capacity. Similar effects of the type of biomass precursor on the H2 S adsorption capacity were observed in other stu-dies using different types of biochar [34,35]
3.3. Effect of impregnation reagent on the adsorption characteristics
Concerning the effect of the type of biomass, the influence of the impregnation reagent on the adsorption efficiency and capacity was investigated. Figure 5shows the adsorption breakthrough curves and removal efficiencies for EUC impregnated with KOH and ZnCl2, respectively. One could clearly see that the adsorption efficiency of EUC is highly affected by the impregnation reagent. The adsorp-tion performance of EUC impregnated with KOH was much better than with ZnCl2. For instance, the breakthrough time with KOH was higher than ZnCl2; it took about 180 min for the H2S outlet concentration to reach its initial value with KOH compared with only 70 min in the case of ZnCl2 (Figure 5). Furthermore, the KOH rendered higher adsorption capacity compared with ZnCl2.
The effect of the impregnation reagent on the breakthrough capacity and adsorption efficiencies can be ascribed to the difference in chemical affi-nity between the properties of H2S in the gas phase and the impregnation reagent. The adsorption of H2S is usually governed by local pH within the pores of the AC, as suggested in the literature . An alkaline pore media, as in the case of KOH, promotes the formation of elemental sulfur through the reaction with the OH group , Equation (10), which increases the H2S removal efficiency. On the other hand, the acidic media, as in the case of ZnCl2, limits the dissociation of H2S; which consequently limits its oxidation to elemen-tal sulfur and thereby reduces the overall H2 S removal [36,38]. In addition, the impregnation reagent also affects the porosity of the AC. Previous studies have indicated that ZnCl2 creates mesoporous structure within the AC, whereas KHO is favorable for creating microporous AC which is generally better for adsorption .
H2Sþ2OH !S2þ2H2O (10)
3.4. Effect of bed height on the adsorption characteristics
To study the effect of the bed height, the adsorp-tion bed was charged with COF AC at different heights of 2, 4, 6 and 8 cm, respectively. The obtained adsorption breakthrough curves are shown in Figure 6. The results indicated that the
0 0.2 0.4 0.6 0.8 1 0 40 80 120 160 200 c/c o of H 2 S Time (min) Euc-KOH Euc-ZnCl2
Figure 5.Breakthrough curves of H2S adsorption in bed packed of EUC-KOH and EUC-ZnCl2. The experiments were performed at
higher the bed height, the higher the adsorption efficiency and the longer the time required for the saturation of the AC. For instance, at a bed height of 2 cm, the c/coratio increased rapidly from 0 to 1 within about 10 min and this time gradually increased with increasing the bed height to reach about 170 min at a bed height of 8 cm. Increasing the bed height means charging the bed with larger amount of AC and consequently increasing the total surface area and the total number of adsorp-tion active sites. Furthermore, a longer AC bed provides a longer contact time between the adsor-bent and the adsorbate, which increases the the amount of adsorbed H2S, as shown inFigure 7.
Future studies should focus on the following aspects in order to upgrade lab-scale studies to pilot and semi-industrial scale experiments: (i) to determine the performance of adsorption columns under the influence of a mixture of pollutants that represents the typical composition of biogas (i.e. H2S, CO2, water vapor, siloxane, O2, CH4 and impurities such as siloxane), (ii) understand the mechanism of adsorption such as electrostatic attraction, interaction between the pollutant and the active sites, and partition in non-carbonized portion of the adsorbents, (iii) perform long-term adsorption studies in continuous systems and identify the deterioration of adsorption capacity
0 0.2 0.4 0.6 0.8 1 0 40 80 120 160 200 c/c o of H 2 S Time (min) 2 cm 4 cm 6 cm 8 cm
Figure 6.Adsorption breakthrough curves of H2S adsorption in packed bed of COF activated with KOH. The experiments were
performed at ambient air temperature, gas flow rate of 1.7 L/min, pressure drop of 9.36 kpa/m, H2S inlet concentration (930 ppm)
and bed heights of 2, 4, 6 and 8 cm.
0 0.06 0.12 0.18 0.24 0.3 0 2 4 6 8 10 Amount adsorbed (g H 2 S) Bed height (cm)
of adsorbents under the influence of changing moisture contents of the biogas.
3.5. Mechanism of H2S removal
In nature, bacterial species could convert the dif-ferent species of sulfur into elemental sulfur after complete oxidation. However, this also depends on the different phases of the sulfur cycle, and the environmental conditions such as pH, tempera-ture, the presence of other competing ions and also on the aerobic, anoxic or anaerobic zones. However, in the case of adsorption-based mechan-isms, the pattern of H2S removal might change depending on the present of sulfur compounds in the gas or liquid phase. Xu et al.  studied the H2S sorption capacities of pig manure and sewage sludge derived biochar for both static and dynamic systems, and revealed that the partial oxidation of H2S into elemental sulfur (S0) takes place in the biochar pores, while complete oxidation of H2 S into sulfate ion (SO42-) occurs on the surface of biochar. The authors also concluded that high moisture content in biochar would accelerate the complete oxidation of H2S, strong alkalinity of biochar helps to achieve high H2S sorption ability, and mineral-rich biochar performs key roles in the conversion of final sulfur compound. Xu et al.  proposed the following H2S removal mechanism (Equations (11)–(15)) by pig manure and sewage sludge derived biochar:
H2Sðgas phaseÞ ! H2Sðadsorbed phaseÞ
! H2Sðliquid phaseÞ (11)
!HSðadsorbed phaseÞþH2O (12)
HSðadsorbed phaseÞþO2! S0 (13)
!SO42ðmajor in pig manure biocharÞ
!CaSO42H2O major in sewage sludge biocharð Þ
3.6. Performance of different adsorbents and practical applications
Based on the literature review, woodchips derived biochar were found to be efficient for the removal of H2S (removal efficiency > 98%) at initial H2 S concentration of 105, 510 and 1020 ppmv, pH 8.0, and moisture content in the range of 80–85% . Agricultural or forest waste such as rice hull, bamboo, camphor tree can be used as a valuable source to produce biochar because of their high H2 S adsorption capacity. However, the adsorption capacity depends on pyrolysis temperature and pH, for example, breakthrough time of an adsorbent increases with the increase of pyrolysis temperature . According to Fellah , different zeolite-based adsorbents can also be used for the removal of gas phase H2S. The important features of this adsorbent can be stated as follows: (i), high surface area, (ii) very high adsorption capacity, (iii) good selectivity, (iv) regenerability and (v) good resistance to high temperatures that are usually expected in industrial emissions. In another recent study, Hassankiadeh and Hallajisani , tested the performance of Molybdenum oxide nano-particles for H2S removal wherein the parameters such as temperature (65–89° C), pressure (10–19 bar), initial concentration of H2 S in the gas phase (38–73 ppm), and space velocity (0.018–0.045 m s−1) were varied. The results from that study showed a maximum adsorption capacity of 0.081 and 0.074 g H2S/g Molybdenum oxide using non-spherical and spherical Molybdenum oxide sor-bent, respectively. In another study involving packed bed systems, Coenen et al.  studied the adsorp-tion behavior of H2S and the influence of steam using commercially available potassium-promoted hydrotalcite. Based on the results obtained from packed bed systems, the authors showed that the operating temperature during adsorption has signif-icant effect on the adsorption behavior. At high and low temperatures (i.e. 500°C and 300°C), different adsorption mechanisms namely chemisorption mechanism with high activation energy and physical
adsorption were reported. It has also been reported that the carbonization temperatures could signifi-cantly affect the surface properties of an adsorbent. Wang et al. , modified the properties of activated carbon samples using a carbonization temperature of 450°C and KOH activation at 750 °C. For H2 S removal, the authors reported a maximum adsorp-tion capacity of ~98.0 mg/g, and the Langmuir iso-therm model was found to describe the mechanism of adsorption of H2S.
From a practical application viewpoint, the effi-cient operation of a biofilter depends on the selec-tion of a proper packing material  as well as the characteristics (e.g. porosity, water retention capability, capacity to hold microbial community) of the selected support media . Compost bio-filter is considered as one of the key biological processes to treat waste gases and to control odor. However, the performance of any compost-based biofilter depends on factors such as the type of filter media, gas flow rate, solubility of the pollutants, its concentration and biodegradability of the substrate [48–50]. As there is very limited information in the literature about effectiveness of biochar-based biofilter for H2S and volatile organic compounds (VOC) removal, future studies should focus on designing reactors using packing materi-als such as Eucalyptus, almond shells and coffee grains and evaluate the performance of these reac-tors in terms of the following parameters: (i) elim-ination capacity, (ii) critical inlet loading rate, (iii) maximum tolerable pollutant concentrations, (iv) capacity to handle transient or shock loads of H2 S and VOCs and (v) perform intelligent control operation of the reactor using artificial intelligence techniques.
The results of this study confirm that AC could be successfully synthesized from various types of locally available biomass wastes and they are tech-nically effective in purifying biogas from H2S. The yield of carbonization was dependent on the type of biomass; i.e. EUC rendered the highest yield of 35% followed by ALM (28%) and COF (23%), respectively. The type of biomass precursor, impregnation reagent and bed height strongly affected the removal efficiency of H2S. The highest
adsorption capacity and removal efficiencies were obtained with EUC followed by ALM and COF, respectively. As an impregnation reagent, KOH gave the higher adsorption efficiency and capacity than ZnCl2. Increasing the bed height increases the adsorption capacity and H2S removal efficiency. Based on the obtained results, for Palestine and other developing countries, it is recommended to use EUC biochar impregnated with KOH for achieving high H2S removal efficiency from the biogas.
● Hydrogen sulfide (H2S) removal by adsorp-tion from biogas was tested in this study ● Effect of the type of precursors, impregnation
reagent and bed height was studied
● KOH activated packing material showed good adsorption efficiency and capacity
● Increasing the bed height increased the H2 S removal efficiency in the packed bed
The authors would like to thank the Palestine Polytechnic University for partially funding this research. The authors also express their thanks to Al-Jebrini Dairy & Food Industry Co. for the use of their biogas facility during long-term reactor experiments. Eldon R. Rene thanks IHE Delft (The Netherlands) for providing staff time and infrastructural support to collaborate with researchers from Palestine.
No potential conflict of interest was reported by the authors.
Hassan Sawalha http://orcid.org/0000-0002-7836-6913
 Liu S, Yang G, Fu J, et al. Synchronously enhancing biogas production, sludge reduction, biogas desulfuri-zation, and digestate treatment in sludge anaerobic digestion by adding K2FeO4. Environ Sci Pollut Res. 2018;25(35):35154–35163.
 Rahman KM, Harder M, Woodard R. Energy yield potentials from the anaerobic digestion of common
animal manure in Bangladesh. Energy Environ.
 Rusmanis D, O’Shea R, Wall DM, et al. Biological hydrogen methanation systems–an overview of design and efficiency. Bioengineered.2019;10(1):604–634.  Koyande AK, Show P-L, Guo R, et al. Bio-processing of
algal bio-refinery: a review on current advances and future perspectives. Bioengineered.2019;10(1):574–592.  Wainaina S, Kumar Awasthi, Taherzadeh MJ.
Bioengineering of anaerobic digestion for volatile fatty acids, hydrogen or methane production: A critical review. Bioengineered.2019;10(1):437–458.  Verma S, Das LM, Kaushik SC. Effects of varying
com-position of biogas on performance and emission charac-teristics of compression ignition engine using exergy analysis. Energy Convers Manag.2017;138:346–359.  Nabais JMV, Laginhas CEC, Carrott PJM, et al.
Production of activated carbons from almond shell. Fuel Process Technol.2011;92(2):234–240.
 Yuan J, Du L, Li S, et al. Use of mature compost as filter media and the effect of packing depth on hydrogen sulfide removal from composting exhaust gases by biofiltration. Environ Sci Pollut Res.2019;26(4):3762–3770.
 Awe OW, Zhao Y, Nzihou A, et al. A review of biogas utilisation, purification and upgrading technologies. Waste Biomass Valorization.2017;8(2):267–283.  Shen M, Zhang Y, Hu D, et al. A review on removal of
siloxanes from biogas: with a special focus on volatile methylsiloxanes. Environ Sci Pollut Res. 2018;25(31) 1–16.
 Tilahun E, Sahinkaya E, Çalli B. A hybrid membrane gas absorption and bio-oxidation process for the removal of hydrogen sulfide from biogas. Int Biodeterior Biodegrad.
 Khoshnevisan B, Tsapekos P, Alfaro N, et al. A review on prospects and challenges of biological H2S removal
from biogas with focus on biotrickling filtration and microaerobic desulfurization. Biofuel Res J. 2017;4 (4):741–750.
 Koparal A, Un UT, Ogutveren UB. Electrochemical oxidation of sulfite ions in aqueous solutions. Int J Environ Pollut.2004;21(6):579–587.
 Biswas RA, Pandey RA, Chakrabarti T, et al. A chemo-biological treatment of scrubbing water from power plants with recovery of value-added products. Int J Environ Pollut.2010;43(1/2/3):129–142.
 Peluso A, Gargiulo N, Aprea P, et al. Nanoporous materials as H2S adsorbents for biogas purification: a
review. Sep Purif Rev.2019;48(1):78–89.
 Binh HTT, Long NQ. Selective adsorption of H2S in
biogas using zeolite prepared by microwave-assisted method. Energy.2016;52:56.
 Machač P, Martinec M. High-temperature separation of H2S from producer gas produced of biomass
gasifi-cation by artificially prepared sorbents. In J Environ Sci Technol.2018;16(8):3971–3978.
 Piergrossi V, Fasolato C, Capitani F, et al. Application of Raman spectroscopy in chemical investigation of impregnated activated carbon spent in hydrogen sul-fide removal process. Int J Environ Sci Technol.
 Wang S, Nam H, Nam H. Utilization of cocoa activated carbon for trimethylamine and hydrogen sulfide gas removals in a confined space and its techno-economic analysis and life-cycle analysis. Environ Prog Sustain Energy.2019;38(6):e13241
 Mohammadi A, Saadati Z, Joohari S. Comparison of the adsorption of H2S by ZnO-TiO2and Ni-ZnO-TiO2
nanoparticles: an adsorption isotherm and thermody-namic study. Environ Prog Sustain Energy. 2019;38(6): e13258
. Ahmad A, Reddy SS. Performance evaluation of upflow anaerobic sludge blanket reactor using immobilized ZnO nanoparticle enhanced continuous biogas production. Energy Environ.2019; 31(2):330–347.  Sathya Priya D, Sureshkumar MV. Synthesis of
Borassus flabellifer fruit husk activated carbon filter for phenol removal from wastewater. Int J Environ Sci Technol.2019; 17(2):829–842
 Rodriguez Correa C, Hehr T, Voglhuber-Slavinsky A, et al. Pyrolysis vs. hydrothermal carbonization: understanding the effect of biomass structural components and inorganic compounds on the char properties. J Anal Appl Pyrolysis.
 Nor NM, Lau LC, Lee KT, et al. Synthesis of activated carbon from lignocellulosic biomass and its applica-tions in air pollution control—a review. J Environ Chem Eng.2013;1(4):658–666.
 Abdullah NS, Hussin MH, Sharifuddin SS, et al. Preparation and characterization of activated carbon fromMoringa Oleiferaseed pod. Cellulose.2017;28:50.  Ho N. Modeling hydrogen sulfide adsorption by acti-vated carbon made from anaerobic digestion by-product. 2012;University of Toronto, Toronto, Canada, Master's Thesis.
 Ioannidou O, Zabaniotou A. Agricultural residues as precursors for activated carbon production—A review. Renew Sust Energ Rev.2007;11(9):1966–2005.  Tripathi M, Sahu JN, Ganesan P. Effect of process
parameters on production of biochar from biomass waste through pyrolysis: A review. Renew Sust Energ Rev.2016;55:467–481.
 Zhong W, Zhang Z, Luo Y, et al. Effect of biological pre-treatments in enhancing corn straw biogas production. Bioresour Technol.2011;102(24):11177–11182.
 Rhodes MJ, Rhodes M. Introduction to particle tech-nology. West Sussex, England:John Wiley & Sons;
 Bear J. Dynamics of fluids in porous media. New York, NY:Courier Corporation;2013.
 Dutt D, Tyagi C. Comparison of various eucalyptus species for their morphological, chemical, pulp and
paper making characteristics. Indian J Chem Technol.
 Ballesteros LF, Teixeira JA, Mussatto SI. Chemical, functional, and structural properties of spent coffee grounds and coffee silverskin. Food Bioprocess Technol.2014;7(12):3493–3503.
 Shang G, Li Q, Liu L, et al. Adsorption of hydrogen sulfide by biochars derived from pyrolysis of different agricultural/forestry wastes. J AirWaste Manage Assoc.
 Sethupathi S, Zhang M, Rajapaksha A, et al. Biochars as potential adsorbers of CH4, CO2 and H2S.
 Adib F, Bagreev A, Bandosz TJ. Effect of pH and surface chemistry on the mechanism of H2S removal by activated
carbons. J Colloid Interface Sci.1999;216(2):360–369.  Turk A, Sakalis E, Rago O, et al. Activated carbon
systems for removal of light gases. Ann N Y Acad Sci.1992;661(1 Frontiers of):221–228.
 Bandosz TJ. On the Adsorption/oxidation of hydrogen sulfide on activated carbons at ambient temperatures. J Colloid Interface Sci.2002;246(1):1–20.
 Okhovat A, Ahmadpour A. A comparative study of the effects of different chemical agents on the pore-size distributions of macadamia nutshell-based activated carbons using different models. Adsorpt Sci Technol.
 Xu X, Cao X, Zhao L, et al. Comparison of sewage sludge- and pig manure-derived biochars for hydrogen sulfide removal. Chemosphere.2014;111:296–303.  Kanjanarong J, Giri BS, Jaisi DP, et al. Removal of
hydro-gen sulfide hydro-generated during anaerobic treatment of sulfate-laden wastewater using biochar: evaluation of effi-ciency and mechanisms. Bioresour Technol. 2017;234: 115–121.
 Fellah MF. Adsorption of hydrogen sulfide as initial step of H2S removal: A DFT study on metal exchanged ZSM-12
clusters. Fuel Process Technol.2016;144:191–196.  Hassankiadeh MN, Hallajisani A. Application of
Molybdenum oxide nanoparticles in H2S removal
from natural gas under different operational and geo-metrical conditions. J Pet Sci Eng.2020;190:107131.  Coenen K, Gallucci F, Hensen E, et al. Adsorption
beha-vior and kinetics of H2S on a potassium-promoted
hydrotalcite. Int J Hydrogen Energy. 2018;43(45): 20758–20771.
 Wang S, Nam H, Nam H. Preparation of activated carbon from peanut shell with KOH activation and its application for H2S adsorption in confined space.
J Environ Chem Eng.2020;8(2):103683.
 Jaber MB, Couvert A, Amrane A, et al. Removal of hydro-gen sulfide in air using cellular concrete waste: biotic and abiotic filtrations. Chem Eng J.2017;319:268–278.  Baltrėnaitė E, Baltrėnas P, Bhatnagar A, et al.
A multicomponent approach to using waste-derived biochar in biofiltration: A case study based on dissim-ilar types of waste. Int Biodeterior Biodegrad.
 Morgan-Sagastume JM, Noyola A. Hydrogen sulfide removal by compost biofiltration: effect of mixing the filter media on operational factors. Bioresour Technol.
 Rene ER, Kar S, Krishnan J, et al. Start-up, perfor-mance and optimization of a compost biofilter treating gas-phase mixture of benzene and toluene. Bioresour Technol.2015;190:529–535.
 Rene ER, Sergienko N, Goswami T, et al. Effects of concentration and gas flow rate on the removal of gas-phase toluene and xylene mixture in a compost biofilter. Bioresour Technol.2018;248(Part B):28–35.